Low-dimensional electronic systems have traditionally been obtained by electrostatically confining electrons, either in heterostructures or in intrinsically nanoscale materials such as single molecules, nanowires and graphene. Recently, a new method has emerged with the recognition that symmetry-protected topological (SPT) phases1,2, which occur in systems with an energy gap to quasiparticle excitations (such as insulators or superconductors), can host robust surface states that remain gapless as long as the relevant global symmetry remains unbroken. The nature of the charge carriers in SPT surface states is intimately tied to the symmetry of the bulk, resulting in one- and two-dimensional electronic systems with novel properties. For example, time reversal symmetry endows the massless charge carriers on the surface of a three-dimensional topological insulator with helicity, fixing the orientation of their spin relative to their momentum3,4. Weakly breaking this symmetry generates a gap on the surface5, resulting in charge carriers with finite effective mass and exotic spin textures6. Analogous manipulations have yet to be demonstrated in two-dimensional topological insulators, where the primary example of a SPT phase is the quantum spin Hall state7,8. Here we demonstrate experimentally that charge-neutral monolayer graphene has a quantum spin Hall state9,10 when it is subjected to a very large magnetic field angled with respect to the graphene plane. In contrast to time-reversal-symmetric systems7, this state is protected by a symmetry of planar spin rotations that emerges as electron spins in a half-filled Landau level are polarized by the large magnetic field. The properties of the resulting helical edge states can be modulated by balancing the applied field against an intrinsic antiferromagnetic instability11,12,13, which tends to spontaneously break the spin-rotation symmetry. In the resulting canted antiferromagnetic state, we observe transport signatures of gapped edge states, which constitute a new kind of one-dimensional electronic system with a tunable bandgap and an associated spin texture14.
This is a preview of subscription content, access via your institution
Open Access articles citing this article.
Quantum Frontiers Open Access 15 November 2022
Nature Communications Open Access 07 September 2021
Nature Communications Open Access 30 July 2021
Subscribe to Journal
Get full journal access for 1 year
only $3.90 per issue
All prices are NET prices.
VAT will be added later in the checkout.
Tax calculation will be finalised during checkout.
Get time limited or full article access on ReadCube.
All prices are NET prices.
Ryu, S., Schnyder, A. P., Furusaki, A. & Ludwig, A. W. W. Topological insulators and superconductors: tenfold way and dimensional hierarchy. N. J. Phys. 12, 065010 (2010)
Chen, X., Gu, Z.-C., Liu, Z.-X. & Wen, X.-G. Symmetry-protected topological orders in interacting bosonic systems. Science 338, 1604–1606 (2012)
Hasan, M. Z. & Kane, C. L. Topological insulators. Rev. Mod. Phys. 82, 3045–3067 (2010)
Qi, X.-L. & Zhang, S.-C. Topological insulators and superconductors. Rev. Mod. Phys. 83, 1057–1110 (2011)
Chen, Y. L. et al. Massive Dirac fermion on the surface of a magnetically doped topological insulator. Science 329, 659–662 (2010)
Xu, S.-Y. et al. Hedgehog spin texture and Berry’s phase tuning in a magnetic topological insulator. Nature Phys. 8, 616–622 (2012)
König, M. et al. Quantum spin Hall insulator state in HgTe quantum wells. Science 318, 766–770 (2007)
Du, L., Knez, I., Sullivan, G. & Du, R.-R. Observation of quantum spin Hall states in InAs/GaSb bilayers under broken time-reversal symmetry. Preprint at http://arxiv.org/abs/1306.1925 (2013)
Abanin, D. A., Lee, P. A. & Levitov, L. S. Spin-filtered edge states and quantum Hall effect in graphene. Phys. Rev. Lett. 96, 176803 (2006)
Fertig, H. A. & Brey, L. Luttinger liquid at the edge of undoped graphene in a strong magnetic field. Phys. Rev. Lett. 97, 116805 (2006)
Herbut, I. F. Theory of integer quantum Hall effect in graphene. Phys. Rev. B 75, 165411 (2007)
Jung, J. & MacDonald, A. H. Theory of the magnetic-field-induced insulator in neutral graphene sheets. Phys. Rev. B 80, 235417 (2009)
Kharitonov, M. Phase diagram for the ν = 0 quantum Hall state in monolayer graphene. Phys. Rev. B 85, 155439 (2012)
Kharitonov, M. Edge excitations of the canted antiferromagnetic phase of the ν = 0 quantum Hall state in graphene: a simplified analysis. Phys. Rev. B 86, 075450 (2012)
Hsieh, T. H. et al. Topological crystalline insulators in the SnTe material class. Nature Commun. 3, 982 (2012)
Kindermann, M. Topological crystalline insulator phase in graphene multilayers. Preprint at http://arxiv.org/abs/1309.1667 (2013)
Min, H. et al. Intrinsic and Rashba spin-orbit interactions in graphene sheets. Phys. Rev. B 74, 165310 (2006)
Semenoff, G. W. Condensed-matter simulation of a three-dimensional anomaly. Phys. Rev. Lett. 53, 2449–2452 (1984)
Checkelsky, J. G., Li, L. & Ong, N. P. Zero-energy state in graphene in a high magnetic field. Phys. Rev. Lett. 100, 206801 (2008)
Yang, K., Das Sarma, S. & MacDonald, A. H. Collective modes and skyrmion excitations in graphene SU(4) quantum Hall ferromagnets. Phys. Rev. B 74, 075423 (2006)
Alicea, J. & Fisher, M. P. A. Graphene integer quantum Hall effect in the ferromagnetic and paramagnetic regimes. Phys. Rev. B 74, 075422 (2006)
Nomura, K., Ryu, S. & Lee, D.-H. Field-induced Kosterlitz-Thouless transition in the N = 0 Landau level of graphene. Phys. Rev. Lett. 103, 216801 (2009)
Young, A. F. et al. Spin and valley quantum Hall ferromagnetism in graphene. Nature Phys. 8, 550–556 (2012)
Maher, P. et al. Evidence for a spin phase transition at charge neutrality in bilayer graphene. Nature Phys. 9, 154–158 (2013)
Mazo, V., Huang, C.-W., Shimshoni, E., Carr, S. T. & Fertig, H. A. Superfluid-insulator transition of quantum hall domain walls in bilayer graphene. Preprint at http://arxiv.org/abs/1309.1563. (2013)
Roth, A. et al. Nonlocal transport in the quantum spin Hall state. Science 325, 294–297 (2009)
Büttner, B. et al. Single valley Dirac fermions in zero-gap HgTe quantum wells. Nature Phys. 7, 418–422 (2011)
Shitade, A. et al. Quantum spin Hall effect in a transition metal oxide Na2IrO3 . Phys. Rev. Lett. 102, 256403 (2009)
Abanin, D. A. & Levitov, L. S. Conformal invariance and shape-dependent conductance of graphene samples. Phys. Rev. B 78, 035416 (2008)
Marchenko, D. et al. Giant Rashba splitting in graphene due to hybridization with gold. Nature Commun. 3, 1232 (2012)
Hunt, B. et al. Massive Dirac fermions and Hofstadter butterfly in a van der Waals heterostructure. Science 340, 1427–1430 (2013)
Dean, C. R. et al. Boron nitride substrates for high-quality graphene electronics. Nature Nanotechnol. 5, 722–726 (2010)
Jalilian, R. et al. Scanning gate microscopy on graphene: charge inhomogeneity and extrinsic doping. Nanotechnology 22, 295705 (2011)
Goossens, A. M. et al. Mechanical cleaning of graphene. Appl. Phys. Lett. 100, 073110 (2012)
Ashoori, R. C. et al. Single-electron capacitance spectroscopy of discrete quantum levels. Phys. Rev. Lett. 68, 3088–3091 (1992)
Goodall, R. K., Higgins, R. J. & Harrang, J. P. Capacitance measurements of a quantized two-dimensional electron gas in the regime of the quantum Hall effect. Phys. Rev. B 31, 6597–6608 (1985)
We acknowledge discussions with D. Abanin, A. Akhmerov, C. Beenakker, L. Brey, L. Fu, M. Kharitonov, L. Levitov, P. Lee and J. Sau. B.H. and R.C.A. were funded by the BES Program of the Office of Science of the US DOE, contract no. FG02-08ER46514, and the Gordon and Betty Moore Foundation, through grant GBMF2931. J.D.S.-Y, and P.J.-H. were primarily supported by the US DOE, BES Office, Division of Materials Sciences and Engineering, under award DE-SC0001819. Early fabrication feasibility studies were supported by NSF Career Award no. DMR-0845287 and the ONR GATE MURI. This work made use of the MRSEC Shared Experimental Facilities supported by the NSF under award no. DMR-0819762 and of Harvard’s CNS, supported by the NSF under grant no. ECS-0335765. Some measurements were performed at the National High Magnetic Field Laboratory, which is supported by NSF Cooperative Agreement DMR-0654118, the State of Florida and the DOE. A.F.Y. acknowledges the support of the Pappalardo Fellowship in Physics.
The authors declare no competing financial interests.
Extended data figures and tables
False-colour AFM images of the devices enumerated in Extended Data Table 1. Dashed lines outline the graphene boundary. Black scale bars correspond to 1 μm.
Colouring of lines from blue to red indicates increasing BT, with B⊥ as indicated at the top of each panel.
Correspondingly higher values of BT are required to induce the transition for higher values of B⊥. For device A, the curves correspond to B⊥ = 0.75, 1, 1.2, 1.4, 1.6, 2, 2.5, 3, 3.5 and 4 T (blue to red). For device B, the curves correspond to B⊥ = 1, 1.5, 2, 2.5, 3 and 3.5 T (blue to red). For device E, the curves correspond to B⊥ = 0.9, 1, 1.1, 1.2, 1.3, 1.4 and 1.5 T (blue to red).
In the main text, evidence for conduction via edge states in the QSH and CAF regimes is provided by non-local transport measurements in device A (Figs 2b and 4b). Owing to conduction through counterpropagating edge states, interrupting an edge with a floating contact decreases the two-terminal conductance much more than would be expected in a diffusive transport model. Here we provide an additional example of this behaviour for device C. a, Schematic of distinct two-terminal measurement topologies with different numbers of floating contacts (open circles). b, QSH regime, B⊥ = 2.7 T and BT = 45 T. c, CAF regime, B⊥ = 5.9 T and BT = 45 T. Curves are colour-coded according to the measurement schematics, as in the main text. Owing to a small gate leak in one of the contacts, these specific non-local measurements underestimate the conductance by a scale factor that was adjusted for by fitting the ν = −1 plateau to a conductance of e2/h.
A generic feature of the intermediate regime between the insulating and metallic QSH regimes is the appearance of double conductance peaks close to ν = 0. The figure shows two-terminal conductance versus back-gate voltage, VG. Purely perpendicular magnetic field only (BT = B⊥, black lines) results in an insulating state at ν = 0. Increasing the total magnetic field while keeping the perpendicular component constant (BT > B⊥, red lines), induces a transition to the CAF with an associated double conductance peak feature. Devices are ordered from left to right by descending aspect ratio.
Extended Data Figure 6 Temperature dependence of the charge-neutrality point conductivity for device B.
a–c, Gate sweeps for device B at constant B⊥ = 2.5 T and BT = 2.5 (a), 26.5 (b) and 34.5 T (c). d, Conductance at the charge-neutrality point as a function of temperature for the data in a–c. A clear insulating dependence (∂G/∂T > 0) is observed for B⊥ = BT. With increased BT, in the intermediate regime, the double conductance peaks between ν = 0 and ν = ±1 have a weakly metallic temperature dependence (∂G/∂T < 0) whereas Gcnp is very weakly insulating. In the QSH regime (BT B⊥), where the conduction is along edge channels, the temperature dependence at ν = 0 is metallic.
Extended Data Figure 7 Schematic diagram of the capacitance bridge-on-a-chip in a tilted magnetic field.
The magnetic field points up in the diagram. Beige: sample stage, showing axis of rotation (red arrows). Purple: graphene sample mount. Blue: transistor mount with 90° bend. The HEMT is mounted on the face angled at 90° to the graphene sample mount and with the plane of its 2D conduction channel perpendicular to the sample-stage axis of rotation. A single wire bond connects the two mounts, from the graphite back gate to the balance point of the capacitance bridge. The transistor is gated by applying VG to the balance point/graphite back gate through a 100-MΩ chip resistor. Combined with the total capacitance of the balance point to ground (∼3 pF), this sets the low-frequency cut-off for the measurement at ∼1 kHz. The density of electrons in the graphene sample is determined by the d.c. voltage difference between the graphene sample and the graphite back gate, namely by Vs − VG. In the main text, this is compensated for and all capacitance measurements are shown as functions of the graphite gate voltage relative to grounded graphene. All components shown in black are at room temperature.
In a fraction of devices with the same geometry as those discussed in the main text, we find that, rather than a conductivity of ∼e2/h at charge neutrality, these devices instead have insulating behaviour at the charge-neutrality point at zero applied magnetic field. We ascribe this insulating behaviour to the opening of a bandgap at the charge-neutrality point owing to the effect of an aligned hBN substrate31. The top panel shows the resistance of the device in zero magnetic field. This device has a resistance of 825 kΩ at the charge-neutrality point in zero magnetic field and at T = 0.3 K. As with the devices described in the main text, the insulating state becomes stronger in a perpendicular magnetic field. In the bottom panel, solid lines are gate sweeps at constant B⊥ = 1, 2 and 3 T and BT = B⊥. Dashed lines are for the corresponding sequence with B⊥ = 1, 2 and 3 T but BT = 45 T. Data taken at 0.3 K. Semiconducting graphene samples do not show any sign of QSH-type physics, at least up to 45 T. Even for B⊥ = 1 T and BT = 45 T, the conductance at the charge-neutrality point increases only slightly, from 0.02e2/h with zero in-plane field to 0.14e2/h with BT = 45 T. This is understandable, because, even neglecting interaction effects, closing a moiré-induced band gap of Δ = 10 meV requires a Zeeman field of nearly Δ/gμB ≈ 85 T. We note that in these samples, the ground state at BT = B⊥ may not be an antiferromagnet.
About this article
Cite this article
Young, A., Sanchez-Yamagishi, J., Hunt, B. et al. Tunable symmetry breaking and helical edge transport in a graphene quantum spin Hall state. Nature 505, 528–532 (2014). https://doi.org/10.1038/nature12800
This article is cited by
Quantum Frontiers (2022)
Nature Nanotechnology (2021)
Edge channels of broken-symmetry quantum Hall states in graphene visualized by atomic force microscopy
Nature Communications (2021)